#------------------------------------------------------------------------------
#$Date: 2024-04-05 01:43:12 +0300 (Fri, 05 Apr 2024) $
#$Revision: 290836 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/57/09/1570953.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1570953
loop_
_publ_author_name
'Chen, Liang'
'Cao, Yili'
'Ma, Rui'
'Cao, Hongmei'
'Chen, Xin'
'Lin, Kun'
'Li, Qiang'
'Deng, Jinxia'
'Liu, Chunyu'
'Wang, Yilin'
'Huang, Ling'
'Xing, Xianran'
_publ_section_title
;
 Regulating luminescence thermal enhancement in negative thermal expansion
 metal-organic frameworks.
;
_journal_issue                   10
_journal_name_full               'Chemical science'
_journal_page_first              3721
_journal_page_last               3729
_journal_paper_doi               10.1039/d3sc06710f
_journal_volume                  15
_journal_year                    2024
_chemical_formula_moiety         'C96 Eu12 N12 O64'
_chemical_formula_sum            'C96 Eu12 N12 O64'
_chemical_formula_weight         4168.60
_chemical_name_systematic        3
_space_group_crystal_system      cubic
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_atom_sites_solution_primary     direct
_audit_creation_date             2023-12-05
_audit_creation_method
;
Olex2 1.5
(compiled 2023.08.24 svn.re1ec1418 for OlexSys, GUI svn.r6817)
;
_audit_update_record
;
2023-12-05 deposited with the CCDC.	2024-01-30 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   21.7226(9)
_cell_length_b                   21.7226(9)
_cell_length_c                   21.7226(9)
_cell_measurement_reflns_used    1174
_cell_measurement_temperature    200
_cell_measurement_theta_max      27.4740
_cell_measurement_theta_min      2.6460
_cell_volume                     10250.3(7)
_computing_cell_refinement       'CrysAlisPro 1.171.42.86a (Rigaku OD, 2023)'
_computing_data_collection       'CrysAlisPro 1.171.42.86a (Rigaku OD, 2023)'
_computing_data_reduction        'CrysAlisPro 1.171.42.86a (Rigaku OD, 2023)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2019/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXS  (Sheldrick, 2008)'
_diffrn_ambient_temperature      200.00
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 0.941
_diffrn_measured_fraction_theta_max 0.934
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω     43.00  69.00   0.50    6.00    --   14.22-132.00-126.00   52
  2  ω    -18.00  20.00   0.50    6.00    --  -17.50 -99.00 -90.00   76
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy R, DW system, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0020428000
_diffrn_orient_matrix_UB_12      0.0290123000
_diffrn_orient_matrix_UB_13      -0.0147524000
_diffrn_orient_matrix_UB_21      -0.0325793000
_diffrn_orient_matrix_UB_22      -0.0021482000
_diffrn_orient_matrix_UB_23      0.0004570000
_diffrn_orient_matrix_UB_31      -0.0005268000
_diffrn_orient_matrix_UB_32      0.0147962000
_diffrn_orient_matrix_UB_33      0.0291486000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0655
_diffrn_reflns_av_unetI/netI     0.0559
_diffrn_reflns_Laue_measured_fraction_full 0.941
_diffrn_reflns_Laue_measured_fraction_max 0.934
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            2048
_diffrn_reflns_point_group_measured_fraction_full 0.941
_diffrn_reflns_point_group_measured_fraction_max 0.934
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.468
_diffrn_reflns_theta_min         2.652
_diffrn_source                   'Rotating-anode X-ray tube'
_diffrn_source_type              'Rigaku (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    3.672
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.71789
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.86a (Rigaku Oxford Diffraction, 2023)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear light colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.351
_exptl_crystal_description       octahedral
_exptl_crystal_F_000             3856
_exptl_crystal_size_max          0.01
_exptl_crystal_size_mid          0.01
_exptl_crystal_size_min          0.01
_refine_diff_density_max         1.157
_refine_diff_density_min         -1.163
_refine_diff_density_rms         0.173
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     33
_refine_ls_number_reflns         609
_refine_ls_number_restraints     13
_refine_ls_restrained_S_all      1.028
_refine_ls_R_factor_all          0.0719
_refine_ls_R_factor_gt           0.0513
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0893P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1324
_refine_ls_wR_factor_ref         0.1442
_reflns_Friedel_coverage         0.000
_reflns_number_gt                435
_reflns_number_total             609
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3sc06710f2.cif
_cod_data_source_block           Eu-NH2-BDC_200K
_cod_depositor_comments
'Adding full bibliography for 1570952--1570966.cif.'
_cod_original_cell_volume        10250.3(13)
_cod_database_code               1570953
_shelx_shelxl_version_number     2019/3
_chemical_oxdiff_formula         'C11 H10 N O'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.964
_shelx_estimated_absorpt_t_min   0.964
_olex2_refinement_description
;
1. Restrained distances
 C3-N1
 1.39 with sigma of 0.01
2. Uiso/Uaniso restraints and constraints
Uanis(C3) \\sim Ueq, Uanis(N1) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
3. Others
 Fixed Sof: N1(0.125)
;
_smtbx_masks_void_probe_radius   1.0
_smtbx_masks_void_truncation_radius 1.2
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.309
_oxdiff_exptl_absorpt_empirical_full_min 0.844
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x, z'
'-x, -y, z'
'y, -x, z'
'x, -z, y'
'x, -y, -z'
'x, z, -y'
'z, y, -x'
'-x, y, -z'
'-z, y, x'
'z, x, y'
'y, z, x'
'-y, -z, x'
'z, -x, -y'
'-y, z, -x'
'-z, -x, y'
'-z, x, -y'
'y, -z, -x'
'y, x, -z'
'-y, -x, -z'
'-x, z, y'
'-x, -z, -y'
'z, -y, x'
'-z, -y, -x'
'x, y+1/2, z+1/2'
'-y, x+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'y, -x+1/2, z+1/2'
'x, -z+1/2, y+1/2'
'x, -y+1/2, -z+1/2'
'x, z+1/2, -y+1/2'
'z, y+1/2, -x+1/2'
'-x, y+1/2, -z+1/2'
'-z, y+1/2, x+1/2'
'z, x+1/2, y+1/2'
'y, z+1/2, x+1/2'
'-y, -z+1/2, x+1/2'
'z, -x+1/2, -y+1/2'
'-y, z+1/2, -x+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, -z+1/2, -x+1/2'
'y, x+1/2, -z+1/2'
'-y, -x+1/2, -z+1/2'
'-x, z+1/2, y+1/2'
'-x, -z+1/2, -y+1/2'
'z, -y+1/2, x+1/2'
'-z, -y+1/2, -x+1/2'
'x+1/2, y, z+1/2'
'-y+1/2, x, z+1/2'
'-x+1/2, -y, z+1/2'
'y+1/2, -x, z+1/2'
'x+1/2, -z, y+1/2'
'x+1/2, -y, -z+1/2'
'x+1/2, z, -y+1/2'
'z+1/2, y, -x+1/2'
'-x+1/2, y, -z+1/2'
'-z+1/2, y, x+1/2'
'z+1/2, x, y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, -z, x+1/2'
'z+1/2, -x, -y+1/2'
'-y+1/2, z, -x+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, -z, -x+1/2'
'y+1/2, x, -z+1/2'
'-y+1/2, -x, -z+1/2'
'-x+1/2, z, y+1/2'
'-x+1/2, -z, -y+1/2'
'z+1/2, -y, x+1/2'
'-z+1/2, -y, -x+1/2'
'x+1/2, y+1/2, z'
'-y+1/2, x+1/2, z'
'-x+1/2, -y+1/2, z'
'y+1/2, -x+1/2, z'
'x+1/2, -z+1/2, y'
'x+1/2, -y+1/2, -z'
'x+1/2, z+1/2, -y'
'z+1/2, y+1/2, -x'
'-x+1/2, y+1/2, -z'
'-z+1/2, y+1/2, x'
'z+1/2, x+1/2, y'
'y+1/2, z+1/2, x'
'-y+1/2, -z+1/2, x'
'z+1/2, -x+1/2, -y'
'-y+1/2, z+1/2, -x'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, -z+1/2, -x'
'y+1/2, x+1/2, -z'
'-y+1/2, -x+1/2, -z'
'-x+1/2, z+1/2, y'
'-x+1/2, -z+1/2, -y'
'z+1/2, -y+1/2, x'
'-z+1/2, -y+1/2, -x'
'-x, -y, -z'
'y, -x, -z'
'x, y, -z'
'-y, x, -z'
'-x, z, -y'
'-x, y, z'
'-x, -z, y'
'-z, -y, x'
'x, -y, z'
'z, -y, -x'
'-z, -x, -y'
'-y, -z, -x'
'y, z, -x'
'-z, x, y'
'y, -z, x'
'z, x, -y'
'z, -x, y'
'-y, z, x'
'-y, -x, z'
'y, x, z'
'x, -z, -y'
'x, z, y'
'-z, y, -x'
'z, y, x'
'-x, -y+1/2, -z+1/2'
'y, -x+1/2, -z+1/2'
'x, y+1/2, -z+1/2'
'-y, x+1/2, -z+1/2'
'-x, z+1/2, -y+1/2'
'-x, y+1/2, z+1/2'
'-x, -z+1/2, y+1/2'
'-z, -y+1/2, x+1/2'
'x, -y+1/2, z+1/2'
'z, -y+1/2, -x+1/2'
'-z, -x+1/2, -y+1/2'
'-y, -z+1/2, -x+1/2'
'y, z+1/2, -x+1/2'
'-z, x+1/2, y+1/2'
'y, -z+1/2, x+1/2'
'z, x+1/2, -y+1/2'
'z, -x+1/2, y+1/2'
'-y, z+1/2, x+1/2'
'-y, -x+1/2, z+1/2'
'y, x+1/2, z+1/2'
'x, -z+1/2, -y+1/2'
'x, z+1/2, y+1/2'
'-z, y+1/2, -x+1/2'
'z, y+1/2, x+1/2'
'-x+1/2, -y, -z+1/2'
'y+1/2, -x, -z+1/2'
'x+1/2, y, -z+1/2'
'-y+1/2, x, -z+1/2'
'-x+1/2, z, -y+1/2'
'-x+1/2, y, z+1/2'
'-x+1/2, -z, y+1/2'
'-z+1/2, -y, x+1/2'
'x+1/2, -y, z+1/2'
'z+1/2, -y, -x+1/2'
'-z+1/2, -x, -y+1/2'
'-y+1/2, -z, -x+1/2'
'y+1/2, z, -x+1/2'
'-z+1/2, x, y+1/2'
'y+1/2, -z, x+1/2'
'z+1/2, x, -y+1/2'
'z+1/2, -x, y+1/2'
'-y+1/2, z, x+1/2'
'-y+1/2, -x, z+1/2'
'y+1/2, x, z+1/2'
'x+1/2, -z, -y+1/2'
'x+1/2, z, y+1/2'
'-z+1/2, y, -x+1/2'
'z+1/2, y, x+1/2'
'-x+1/2, -y+1/2, -z'
'y+1/2, -x+1/2, -z'
'x+1/2, y+1/2, -z'
'-y+1/2, x+1/2, -z'
'-x+1/2, z+1/2, -y'
'-x+1/2, y+1/2, z'
'-x+1/2, -z+1/2, y'
'-z+1/2, -y+1/2, x'
'x+1/2, -y+1/2, z'
'z+1/2, -y+1/2, -x'
'-z+1/2, -x+1/2, -y'
'-y+1/2, -z+1/2, -x'
'y+1/2, z+1/2, -x'
'-z+1/2, x+1/2, y'
'y+1/2, -z+1/2, x'
'z+1/2, x+1/2, -y'
'z+1/2, -x+1/2, y'
'-y+1/2, z+1/2, x'
'-y+1/2, -x+1/2, z'
'y+1/2, x+1/2, z'
'x+1/2, -z+1/2, -y'
'x+1/2, z+1/2, y'
'-z+1/2, y+1/2, -x'
'z+1/2, y+1/2, x'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Eu1 Eu 0.37020(4) 0.000000 0.000000 0.0306(4) Uani 1 8 d S T P . .
O1 O 0.4407(2) 0.0593(2) -0.0593(2) 0.019(2) Uani 1 6 d S T P . .
O2 O 0.3241(4) 0.000000 0.0994(4) 0.069(3) Uani 1 2 d S T P . .
C1 C 0.3449(8) 0.000000 0.1551(8) 0.095(8) Uani 1 4 d S T P . .
C2 C 0.2954(8) 0.000000 0.2046(8) 0.123(10) Uani 1 4 d S T P . .
C3 C 0.2327(10) 0.000000 0.1864(9) 0.133(7) Uani 1 2 d DS TU P . .
N1 N 0.211(2) 0.000000 0.1262(12) 0.070(12) Uani 0.25 2 d DS TU P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Eu1 Eu1 Eu1 60.0 56 170 ?
Eu1 Eu1 Eu1 90.0 170 74_545 ?
Eu1 Eu1 Eu1 60.0 56 74_545 ?
Eu1 Eu1 Eu1 90.0 56 152_554 ?
Eu1 Eu1 Eu1 60.0 74_545 152_554 ?
Eu1 Eu1 Eu1 60.0 170 152_554 ?
O1 Eu1 Eu1 85.84(17) 74_545 170 ?
O1 Eu1 Eu1 85.84(17) 99 152_554 ?
O1 Eu1 Eu1 85.84(17) 172_545 170 ?
O1 Eu1 Eu1 33.09(8) 99 56 ?
O1 Eu1 Eu1 33.09(8) 74_545 152_554 ?
O1 Eu1 Eu1 85.84(17) 99 74_545 ?
O1 Eu1 Eu1 33.09(8) 99 170 ?
O1 Eu1 Eu1 33.09(8) 172_545 56 ?
O1 Eu1 Eu1 85.84(17) 172_545 152_554 ?
O1 Eu1 Eu1 85.84(17) 74_545 56 ?
O1 Eu1 Eu1 33.09(8) . 152_554 ?
O1 Eu1 Eu1 85.85(17) . 74_545 ?
O1 Eu1 Eu1 85.85(17) . 56 ?
O1 Eu1 Eu1 33.09(8) 172_545 74_545 ?
O1 Eu1 Eu1 33.09(8) 74_545 74_545 ?
O1 Eu1 Eu1 33.09(8) . 170 ?
O1 Eu1 O1 65.5(2) 99 172_545 ?
O1 Eu1 O1 99.9(4) 172_545 . ?
O1 Eu1 O1 65.5(2) 99 . ?
O1 Eu1 O1 99.9(4) 99 74_545 ?
O1 Eu1 O1 65.5(2) 172_545 74_545 ?
O1 Eu1 O1 65.5(2) 74_545 . ?
O1 Eu1 O2 77.3(2) 172_545 . ?
O1 Eu1 O2 139.61(13) 172_545 99 ?
O1 Eu1 O2 139.61(13) . 5 ?
O1 Eu1 O2 139.61(13) 74_545 . ?
O1 Eu1 O2 77.3(2) 74_545 99 ?
O1 Eu1 O2 77.3(2) . 99 ?
O1 Eu1 O2 139.61(13) 99 99 ?
O1 Eu1 O2 77.3(2) 99 7 ?
O1 Eu1 O2 77.3(2) 99 . ?
O1 Eu1 O2 139.61(13) 74_545 7 ?
O1 Eu1 O2 139.61(13) . . ?
O1 Eu1 O2 77.3(2) 74_545 5 ?
O1 Eu1 O2 139.61(13) 172_545 7 ?
O1 Eu1 O2 139.61(13) 99 5 ?
O1 Eu1 O2 77.3(2) . 7 ?
O1 Eu1 O2 77.3(2) 172_545 5 ?
O2 Eu1 Eu1 159.9(2) 5 170 ?
O2 Eu1 Eu1 107.30(16) 5 56 ?
O2 Eu1 Eu1 107.30(16) 7 152_554 ?
O2 Eu1 Eu1 69.9(2) 5 74_545 ?
O2 Eu1 Eu1 107.30(16) 5 152_554 ?
O2 Eu1 Eu1 107.30(16) 99 170 ?
O2 Eu1 Eu1 107.30(16) 7 56 ?
O2 Eu1 Eu1 159.9(2) 7 74_545 ?
O2 Eu1 Eu1 159.9(2) 99 56 ?
O2 Eu1 Eu1 107.30(16) . 74_545 ?
O2 Eu1 Eu1 69.9(2) 99 152_554 ?
O2 Eu1 Eu1 69.9(2) 7 170 ?
O2 Eu1 Eu1 159.9(2) . 152_554 ?
O2 Eu1 Eu1 107.30(16) . 170 ?
O2 Eu1 Eu1 69.9(2) . 56 ?
O2 Eu1 Eu1 107.30(16) 99 74_545 ?
O2 Eu1 O2 79.81(18) 5 99 ?
O2 Eu1 O2 130.3(5) 99 . ?
O2 Eu1 O2 130.3(5) 5 7 ?
O2 Eu1 O2 79.81(18) 7 . ?
O2 Eu1 O2 79.81(18) 5 . ?
O2 Eu1 O2 79.81(18) 99 7 ?
Eu1 O1 Eu1 113.81(16) 170 . ?
Eu1 O1 Eu1 113.81(16) 170 152_554 ?
Eu1 O1 Eu1 113.81(16) 152_554 . ?
C1 O2 Eu1 134.7(12) . . ?
O2 C1 O2 131(2) . 167 ?
O2 C1 C2 114.6(11) 167 . ?
O2 C1 C2 114.6(11) . . ?
C3 C2 C1 118.8(13) 167 . ?
C3 C2 C1 118.8(13) . . ?
C3 C2 C3 122(3) . 167 ?
C2 C3 C3 118.8(13) . 23 ?
N1 C3 C2 126(3) . . ?
N1 C3 C3 116(2) . 23 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Eu1 Eu1 3.9876(13) 56 ?
Eu1 Eu1 3.9876(13) 152_554 ?
Eu1 Eu1 3.9876(13) 170 ?
Eu1 Eu1 3.9876(13) 74_545 ?
Eu1 O1 2.380(2) 172_545 ?
Eu1 O1 2.380(2) 99 ?
Eu1 O1 2.380(2) 74_545 ?
Eu1 O1 2.380(2) . ?
Eu1 O2 2.380(8) 7 ?
Eu1 O2 2.380(8) 5 ?
Eu1 O2 2.380(8) . ?
Eu1 O2 2.380(8) 99 ?
O2 C1 1.292(13) . ?
C1 C2 1.52(3) . ?
C2 C3 1.42(2) . ?
C2 C3 1.42(2) 167 ?
C3 C3 1.42(4) 23 ?
C3 N1 1.388(10) . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Eu1 O2 C1 O2 0.000(0) . . . 167 ?
Eu1 O2 C1 C2 180.0 . . . . ?
O2 C1 C2 C3 0.000(1) 167 . . 167 ?
O2 C1 C2 C3 180.000(1) 167 . . . ?
O2 C1 C2 C3 0.000(1) . . . . ?
O2 C1 C2 C3 180.000(1) . . . 167 ?
C1 C2 C3 C3 180.000(1) . . . 23 ?
C1 C2 C3 N1 0.000(1) . . . . ?
C3 C2 C3 C3 0.000(0) 167 . . 23 ?
C3 C2 C3 N1 180.000(1) 167 . . . ?
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 -0.851 -0.509 -0.336 5351.2 1291.3 ?
